SURFACE MORPHOLOGY AND OPTICAL PROPERTIES OF COPPER NITRIDE THIN FILM SYNTHESIZED BY DC SPUTTERING
NURUL SHAHIDA BINTI MA'AJIH
SURFACE MORPHOLOGY AND OPTICAL PROPERTIES OF COPPER NITRIDE THIN FILM SYNTHESIZED BY DC SPUTTERING
NURUL SHAHIDA BINTI MA’AJIH
A dissertation submitted in partial fulfillment of the requirement for the award of the degree of
Master of Science (Physics)
Faculty of Science Universiti Teknologi Malaysia
Specially dedicated to
My beloved husband, En. Hanezan bin Hanaffi
For supporting and encouraging me to believe in myself
My parents, En. Ma’ajih bin Ismail and Pn. Narizan binti Mohd
My parents in law, En. Hanaffi bin Hj. Kesman and Pn. Azizah binti Hj. Muhamad
A strong and gentle soul who taught me to trust in Allah, believe in hard work and that so much could be done with little
My siblings from both families
Mohd Mustakim and Siti Nursabariah, Nurul Shahirah, Nurul Shahizzat
Fakhrul Nazhi and Farah Wahida, Farhan and Siti Suhana, Mohd Hanirulhaidi, Mohd Nurafendi, Rafidi, Rafidah
For understanding and supporting me to achieve my dreams
My lovely daughter, Nur Khairina Syafiqah binti Hanezan
All thanks to Allah SWT, who gave me opportunity and strength to complete this study.
First and foremost, I have to thank my parents for their love and support throughout my life. Thank you both for giving me strength to reach for the stars and chase my dreams. My beloved husband deserves my wholehearted thanks as well. My special thanks also dedicated to my sisters and brothers for their endless love, supporting and encouragement.
Then, I would like to express my deepest appreciation to my supervisor, Dr. Wan Nurulhuda binti Wan Shamsuri for her patience and tolerance in guiding, supporting and helping me throughout this project. A special thanks also goes to my Academic Coordinator (Physics), Assoc Prof Dr. Yusof Munajat whom have guided me in achieving the goal.
My sincere appreciation also extends to all laboratory staff members especially Mr. Keliwon Md. Saroji, Mr. Mohd Nazari Kamarudin, Mrs. Junaidah Saman and Mrs. Radiah Hassan for a lot of assistance provided on various occasions.
The purpose of this research is to study the surface morphology and optical properties of copper nitride thin films. Copper nitride thin films were deposited on corning glass substrates by using DC sputtering technique. Five samples were prepared with five different deposition time to obtain samples of different thicknesses. Ellipsometer was used to measure thickness and refractive index. The surface morphology images were obtained by using Atomic Force Microscopy (AFM). Both transmission spectra and photoluminescence spectrum were obtained from UV-Vis-NIR spectrophotometer and Photoluminescence spectrometer, respectively. The films obtained were yellow to reddish-brown depending on increasing deposition time. The thickness of the samples increased as the deposition time increased. Thicknesses of films, d obtained were in range of 1092.38 nm to 1331.03 nm. Refractive index decreased as deposition times increased. The Atomic Force Microscopy images showed that the films were a smooth morphology and were seen like pyramidal islands when deposition time increased. Transparency of copper nitride thin film was very low in the visible region, but it slowly increased in the infrared range. The absorption coefficient, α of copper nitride thin films increased with increasing of photon energy. The average optical band gap energy, Eg obtained in range of 1.56 eV to 2.06 eV. The best emission peak for maximum
Penyelidikan ini bertujuan untuk mengkaji permukaan morfologi dan sifat optik saput tipis kuprum nitrida. Kuprum nitrida telah dipendapkan pada permukaan substrat kaca dengan menggunakan kaedah percikan arus terus. Lima sampel telah disediakan pada lima masa pemendapan yang berbeza untuk menghasilkan sampel yang mempunyai ketebalan yang berbeza. Ellipsometer digunakan untuk mengukur ketebalan dan indeks biasan saput tipis. Imej 3D morfologi bagi semua sampel diperoleh daripada Atomic Force Microscopy (AFM). Kadar penghantaran sampel diukur dengan menggunakan UV-Vis-NIR Spectrophotometer dan analisis foto luminescence diukur menggunakan Photoluminescence Spectrometer. Saput tipis yang terhasil adalah berwarna coklat kemerahan bergantung kepada masa pemendapan. Ketebalan sampel bertambah apabila masa pemendapan bertambah. Ketebalan filem, d yang terhasil dengan julat antara 1092.38 nm hingga 1331.03 nm. Indeks biasan adalah berkurang apabila ketebalan sampel bertambah. Imej yang dihasilkan oleh AFM adalah permukaan morfologi seragam dan kelihatan seperti piramid apabila masa pemendapan bertambah. Kadar penghantaran kuprum nitrida adalah rendah dalam cahaya nampak, tetapi mula meningkat dalam julat sinar merah. Pekali penyerapan, α bertambah apabila tenaga fonon bertambah. Purata jurang tenaga optik, Eg adalah antara julat 1.56 eV hingga 2.06 eV. Panjang
TABLE OF CONTENTS
CHAPTER TITLE PAGE
TABLE OF CONTENTS vii
LIST OF TABLES x
LIST OF FIGURES xi
LIST OF ABBREVIATIONS xiii
LIST OF SYMBOLS xiv
1.1 Background of research 1
1.2 Problem Statement 3
1.3 Research Objectives 4
1.4 Scope of the Study 4
1.5 Significance of the Study 5
2 LITERATURE REVIEW
2.1 Thin Film 6
2.3 DC Sputtering Process 13
2.4 Optical Properties
2.4.1 Refractive Index, n 2.4.2 Absorption Coefficient, α 2.4.3 Energy Band Gap, Eg
18.104.22.168 Direct and Indirect Band Gap
16 17 18 19 20 2.5 Basic Mechanism of Photoluminescence 21 2.6 Instrumentation of Characterization of Thin Films
2.6.2 Atomic Force Microscopy (AFM) 2.6.3 UV-Vis-NIR Spectrophotometer Measurements
2.6.4 Photoluminescence Spectrometer Measurements
24 25 28
3.1 Sample Preparation 31
3.2 DC Sputtering Deposition 33
3.3 Characterization of Copper Nitride Thin Films 3.3.1 Thickness and Refractive Index
Measurement using Ellipsometer 3.3.2 Surface Morphology and Grain Size Properties by Atomic Force
3.3.3 UV-Vis-NIR Spectrophotometer 3.3.4 Photoluminescence Spectrometer
39 40 3.4 Storage of Copper Nitride Thin Films 40
4 RESULTS AND DISCUSSION
4.2 Thickness, d 43
4.3 Refractive Index, n 45
4.4 Surface Morphology and Grain Size 45
4.5 Transmittance 49
4.6 Absorption Coefficient, α and Optical Band Gap Energy, Eg
4.7 Photoluminescence Spectrum
5 CONCLUSIONS AND SUGGESTIONS
5.1 Conclusions 55
5.2 Suggestions 57
LIST OF TABLES
FIGURE NO. TITLE PAGE
4.1 Thickness, d of samples 44
4.2 Comparison between thickness, d and deposition time of samples
4.3 Relationship between thickness, d and refractive index, n of samples
LIST OF FIGURES
FIGURE NO. TITLE PAGE
2.1 Structure of copper nitride 10
2.2 The copper nitride thin film result for optical properties 12
2.3 The sputter deposition process 15
2.4 Comparison between direct and indirect band gap 21 2.5 The mechanism of photoluminescence process 23 2.6 Rotating analyzer ellipsometer schematic 25
2.7 AFM Diagram 26
3.1 Dimension of glass substrate 32
3.2 Ultrasonic Branson 3210 Cleaner 33
3.3 The schematic diagram of DC sputtering machine 34
3.4 DC sputtering deposition 35
3.5 Flow chart of sample preparation 36
3.6 Ellipsometer 37
3.7 Atomic Force Microscopy (AFM) 39
3.8 UV-Vis-NIR Spectrometer 40
3.9 Perkin Elmer LS55 Luminescence Spectrometer 41
3.10 Desiccators for thin film storage 41
4.1 Samples in reddish-brown colour after deposition process
4.2 3D AFM image of copper nitride thin film at various deposition time
4.3 UV-Vis Transmission spectra of copper nitride thin film prepared at various deposition time
4.4 Absorption coefficient, α at various wavelength, λ 51 4.5 Plot of (αhʋ)½vs hʋ of the copper nitride thin film grown
at different deposition time
4.6 PL emission spectra of copper nitride thin film at five deposition time
LIST OF ABBREVIATIONS
AC - Alternating Current
AES - Auger Electron Spectroscopy AFM - Atomic Force Microscopy
CL - Cathodoluminescence
DC - Direct Current
EL - Electroluminescence
IBAD - Ion Beam Assisted Deposition
NIR - Near Infrared
PL - Photoluminescence
RF - Reactive Frequency
RMS - Root Mean Square
SEM - Scanning Electron Microscopy SPM - Scanning Probe Microscopy
UV - Ultraviolet
VIS - Visible
LIST OF SYMBOLS
A - Absorbance
Ar - Argon
B - Band tailing constant
Cu - Copper
d - Thickness
Eg - Energy band gap
Eopt - Optical band gap energy
I - Intensity
I0 - Intensity of incident light
IA - Intensity of absorbed light
IR - Intensity of reflected light IT - Intensity of transmitted light
N - Nitrogen
n - Refractive index
O - Oxygen
PbS - Plumbum Sulfide
T - Transmittance
α - Absorption coefficient
Ө1 - Angle of incidence
This chapter consists of some general information about background of research definition of thin film, problem statement, research objectives and the scope of the research.
1.1 Background of Research
Any solid or liquid object with one of its dimensions very much less than that of the other two may be called a “thin film” (George, 1996). The most commonly observed phenomenon associated with thin films, which attracted the attention of physicists as early as the second half of seventeenth century, is the fascinating colours on a thin film of oil coating on the surface of water.
stages, scientific interest in thin solid films centered on antireflection coatings for lenses, multilayer interference filters, automobile headlights and decorative coatings.
An application of thin film technology has revolutionized the field of optics and electronics. The need for new and improved optical and electrical devices has stimulated the study of thin solid films of elements, as well as binary and ternary systems, which controlled composition and specific properties, and has consequently accelerated efforts to develop different thin film deposition techniques. Among advantages of thin films devices are low power consumption, relatively small and reduction occupied space and higher speed performance (Sakrani, 2004).
In recent years, copper nitride thin film has been attracting considerable attention as a new material applicable for optical storage devices and high-speed integrated circuits (Maruyama et al., 1996 & Dorranian et al, 2012). It is a promising material for write - once optical recording media devices and microscopic metal links in ultra large scale integrated circuits due to its excellent properties such as nontoxicity and thermal decomposition at lower temperature (100 ~ 470 °C).
It is also an indirect band gap semiconductor with low reﬂectivity and high electrical resistivity at room temperature. Additionally, this material can also be used as the candidates for an insulating barrier in magnetic tunnel junctions and the electrode material of Li-ion batteries (Xing et al., 2007).
have relatively smaller grains. The optical energy gap were measured to be in the range of 1.34 – 1.75 eV.
Many research groups have been synthesized copper nitride thin ﬁlms by various methods, such as molecular beam epitaxial, DC magnetron sputtering, RF magnetron sputtering, pulsed laser deposition, and ion assisted vapor deposition (Arrabal et al., 2010). However, the phenomenon of sputtering has several advantages in film deposition compared to others. There is no direct heating of the material as in evaporation methods.
Therefore, there is no reaction between the source and crucible place. This method is commercially advantageous, since they are relatively easy to scale up, offer high deposition rates, and are comparatively gentle to the substrate (Liljeholm, 2012). The popularity of DC sputtering from elemental targets can be attributed to several factors, like it is capable of producing thin compound films of controllable stoichiometry and composition at high deposition rates and on an industrial scale and high-purity films can be produced due to the elemental targets are usually more easily purified.
1.2 Problem Statement
different deposition times. The surface morphology and optical properties of copper nitride thin films would be investigated.
The objectives of this study are:
1. To synthesize the copper nitride thin film by using DC sputtering method.
2. To determine the surface morphology and grain size of copper nitride thin film by Atomic Force Microscopy (AFM).
3. To characterize the absorption of the copper nitride thin film by means of UV-Vis-NIR spectroscopy.
4. To characterize the emission properties of the copper nitride thin film by means of PL spectroscopy.
1.4Scope of the Study
The scope of study has been focus on following:
2. Determination the thickness and refractive index of copper nitride thin film by using Ellipsometer.
3. Determination of surface morphology and grain size of copper nitride thin film by using Atomic Force Microscopy (AFM).
4. Characterization of transmission spectra by using UV-Vis-NIR spectrophotometer and determination of absorption coefficient and optical band gap energy.
5. Characterization of emission properties by using Photoluminescence spectrometer.
1.5 Significance of the Study
Arrabal, R. G., Gordillo, N., Martin Gonzales, M. S., Ruiz Bustors, R., and Agullo- Lopez, F. (2010). Thermal Stability of Copper Nitride Thin Films: The Role of Nitrogen Migration. Journal of Applied Physics. 107(103513), 1-7.
Barna, P. B. (2005). History of Thin Films: Growth, Techniques, Characterization.
Advanced Materials Science and Electron Microscopy.
Chen, E. (2004). Thin Film Deposition. Applied Physics. 298.
Cho, S. (2012). Effect of substrate temperature on the properties of copper nitride thin films deposited by reactive magnetron sputtering. Current Applied
Physics. 12, 44-47.
Dorranian, D., Dejam, L., Sari, A. H., and Hojabri, A. (2009). Effect of nitrogen Content on Optical Constants of Copper Nitride Thin Films Prepared by DC Magnetron Reactive Sputtering. Journal of Theoretical and Applied Physics. 3-3, 37- 41.
Dorranian, D., Dejam, L., and Mosayebian, G. (2012). Optical characterization of Cu3N thin film with Swanepoel method. Journal of Theoretical and Applied
Physics. 6, 13.
Gallardo-Vega, C., and de la Cruz, W. (2006). Study of the structure and electrical properties of the copper nitride thin films deposited by pulsed laser
deposition. Applied Surface Science. 252, 8001-8004.
George. J., (1996). “Preparation of Thin Film”. United State of America.
Ghosh, S., Singh, F., Choudharya, D., Avasthia, D. K., Ganesanb, V., Shah, P., and Gupta, A. (2001). Effect of substrate temperature on the physical properties of copper nitride films by r.f. reactive sputtering. Surface and Coatings
Technology. 142-144, 1034-1039.
Hayashi, Y., Ishikawa, T., and Shimokawa, D. (2002). Modification of electrical and optical peroperties of metal nitride thin films by hydrogen inclusion.
Journal of Alloys and Compounds. 330 (332), 348 -351.
Hanewald, K., Glutsch, S, and Bechstedt, F. Theory of photoluminescence excitation spectroscopy in semiconductors. Applied Physics.
Ji, A. L., Huang, R., Du, Y., Li, C. R., Wang, Y. Q., and Cao, Z.X. (2006). Growth of stoichiometric Cu3N thin films by reactive magnetron sputtering. Journal
ofCrystal Growth . 295, 79-83.
Lotfi-Kajlahi, A., and Savaloni, H. (2013). Investigation on the production of copper nitride (copper azide) thin films and their nanostructures. Journal of
Theoretical and Applied Physics. 72, 1-6.
Liljeholm, L. (2012). Reactive Sputter Deposition of Functional Thin Films. Digital Comprehensive Summaries of Uppsala Dissertations from the Faculty of
Science and Technology. 945, ISBN 978-91-554-8403-3.
Maruyama, T., and Morishita, T. (1995). Copper Nitride Thin Film Prepared by RF Reactive Sputtering. Journal Applied Physics. 78 (4104).
Maruyama, T., and Morishita, T. (1996). Copper Nitride and Tin Nitride Thin Films forWriteonce Optical Recording Media. Applied Physics Letters. 69(7).
Mech, K., Kowalik, R., and Zabinski, P. (2011). Cu Thin Films Deposited by DC Magnetron Sputtering for Contact Surfaces on Electronic Components.
Mikula, M. (2001). Electrical and Optical Properties of Copper Nitride Thin Films
Prepared By Reactive DC Magnetron Sputtering. 51 (1), 35-43.
Noor Azizun, M. A. Optical properties and Photoluminescence of Copper Nitride
Thin Film prepared by Reactive DC Sputtering. Master of Science Thesis.
Universiti Teknologi Malaysia; 2013.
Nosaka, T., Yoshitake, M., Okamoto, A., Ogawa, S., and Nakayama, Y. (1999). Copper nitride thin films prepared by reactive radio-frequency sputtering.
Thin SolidFilms. 348, 8-13.
Odeh, I. M. (2008). Fabrication and Optical Constants of Amorphous Copper Nitride Thin Films Prepared by Ion Beam Assisted DC Magnetron Reactive Sputtering. Journal of Alloys and Compound. 454, 102-105.
Pierson, J. F. (2002). Structure and properties of copper nitride films formed by reactive magnetron sputtering. Vacuum. 66, 59-64.
Reddy, K. V. S., Reddy, A. S., Reddy, P. S.,and Uthanna, S. (2007). Copper nitride films deposited by dc reactive magnetron sputtering. J Mater Sci: Mater
Sakrani, S. (2004). Lecture Note: Thin Films technology. Universiti Teknologi Malaysia.
Shinde, K.N. (2013). Basic Mechanisms of Photoluminescence. Springer Series in
Materials Science. 174.
Subbareddy, K. V., Subramanyam, K., and Uthanna, S. (2007). Optoelectronics and
Advanced Materials – Rapid Communications. 1 (1), 31-35.
Wang, D. Y., Nakamine, N., Hayashi, Y. (1998). Properties of Various Sputter Deposited Cu-N Thin Films. Journal of Vacuum Science and Technology. 16, 2084-2092.
Wang, J., Chen, J. T., Yuan, X. M., Wu, Z. G., Miao, B. B., and Yan, P. X. (2006). Copper Nitride Thin Films Deposited by RF Magnetron Sputtering. Journal
of Crystal Growth. (286), 407-412.
Xiao, J., Li, Y., and Jiang, A. (2011). Structure, Optical Property and Thermal Stability of Copper Nitride Films Prepared by Reactive Radio Frequency Magnetron Sputtering. J. Mater. Sci. Techno. 27(5), 403-407.
Xing, L., Zuli, L., Anyou, Z., Zuobin, Y., Jianping, Y., and Kailun, Y. (2007). Properties of Al-doped Copper Nitride Films Prepared by Reactive
Magnetron Sputtering. Journal of Wuhan University of Technology Mater Sci. Ed. 22 (3).